Fabrication, Characterization, and Impact of Heat Treatment on Sliding Wear Behaviour of Aluminium Metal Matrix Composites Reinforced with B4C

,e aim of this research paper is to find the wear behaviour of Al7075MMCs. In this investigation, the wear tests on the as-cast and age-hardened specimens were performed on an advanced rotary tribometer.,ematerials selected for the analysis are Al7075 as a matrix, and the reinforcements are boron carbide. By using stir casting, metal matrix composites are manufactured by adding B4C as a reinforcement particulate in Al7075. ,e fabricated composites were characterized and the wear behaviour of these composites was carried out on an advanced rotary tribometer.,ewt. % of the reinforcements was taken as 6%, 8%, 10%, and 12%. ,e almost homogeneous blending of reinforcements is shown by the microstructural characterization of Al7075MMCs. It is observed that due to the rise in weight percentage of the reinforcement to 12% higher hardness is obtained. For 12% of reinforcements, there is an increase in hardness due to the heat treatment than that of the as-cast composites. From this study, it was found that the wear rate is the function of the applied load, microstructure, and volume fraction of the reinforcements. ,e wear rate was increasing with the sliding velocity.


Introduction
In recent years, a lot of research has been carried out for the aluminium matrix composite reinforced with ceramic particulates. In the literature study, it is seen that less work has been carried out regarding the effect of variation of the size of the reinforced particulates. A review on the tribological characterization of particulate reinforced with aluminium metal matrix composites has been published by Shinde et al. [1]. ey reported that there is an increasing trend of using aluminium-based composites in sectors such as ground transportation, aerospace, and sports. ey reported the reasons for using aluminium-based composites as high strength-to-weight ratio, wear resistance, corrosion, and fatigue. Dragut et al. [2] have produced Al/ AlB 2 in situ composites via an exothermic chemical reaction between KBF 4 and liquid AA6060 aluminium alloy at 850°C. e presence of AlB 2 compounds in the composite material was observed using an optical microscope and SEM. e main driving forces for the development of this material were the aerospace and automotive industries for both nonstructural and structural applications. Stoloff and Alman [3] published a research paper on innovative processing techniques for intermetallic matrix composites. ey proposed processing techniques for composites through three routes, powder processing, melt processing, and vapour phase processing. e powder processing technique is consisting of various methods such as reactive consolidation, injection molding, mechanical alloying, XD processing, high energy rate forming, and microstructurally toughened composites. e melt processing technique includes pressure casting and directional solidification of eutectics. e vapour phase processing for composites includes the arc spray method, chemical vapour deposition, filament coating, and lowpressure plasma spray.
Goni et al. [4] developed low-cost metal matrix composites (MMCs) for commercial applications by using locally reinforced aluminium composites and new castable aluminium MMCs. Al6061/WC/SiC hybrid composites have been synthesized using the stir casting technique under the various weight percentages of reinforcement [5]. Various properties such as wear resistance, hardness, tensile strength, and compressive strength were characterized and investigated in this research paper. From the microstructural analysis point of view, they reported that reinforcement particles were uniformly distributed without any clustering in the matrix. ey further reported that precipitates of Mg 2 Si and undissolved Al6 (Fe, Mn) are seen as a result of the interfacial reaction. ey concluded that hardness of the composites has been enhanced. e enhancement in hardness of the composites is due to the incorporation of stronger and stiffer reinforcement in the matrix.
Manivannan et al. [6] fabricated nanocomposites Al6061/nano-SiC by using a liquid metallurgy technique. ey presented the wear characteristics of the fabricated nanocomposites. ey analyzed the worn surfaces as well as wear debris by using FESEM equipped with EDS. ey claimed that the nanocomposite exhibits improved wear resistance as compared to the Al6061 alloy. ey proposed that the worn surface shows different mechanisms such as abrasion, delamination, oxidation, and adhesive wear at different loads. e sliding wear test of Al-SiC and Al-B 4 C composites were performed on a pin-on-disc setup. Shorowordi et al. [7] analyzed the tribo-surface characteristics of the composites worn under different content pressures from 0.75 MPa to 3 MPa at a linear speed. e wear tests were performed against a commercial phenolic brake pad under dry conditions. e investigators recorded the coefficient of friction online. ey characterized the worn surfaces using SEM equipped with EDS. ey found that the wear rate of both the composites was increasing with the increasing contact pressure. ey further reported that the surface roughness of Al-MMCs was increased with increasing contact pressure. For both the composites, the coefficient of friction slightly decreases with the increasing pressure. It was reported that a transfer layer of the phenolic counter body was seen on the pin of Al-MMC, and wear rate and coefficient of friction were higher for Al-SiC as compared to those of Al-B 4 C.
In an investigation, Rajesh et al. [8,9] have analyzed the effect of reinforcing Al 2 O 3 and SiC on the wear behaviour of hybrid aluminium MMCs on a pin-on-disc tribometer. ey fabricated the composites by using the reinforcement SiC with 5%, 10%, and 15% weight and Al 2 O 3 with 5%, 10%, and 15% weight through stir casting. ey reported that microstructural characterization indicates homogeneous mixing of the reinforcements. ey concluded that the wear resistance of the composite was increased due to the addition of SiC and Al 2 O 3 . e wear tests were performed on both as-cast and age-hardened composites. ey found that the rate of wear was reduced either by increasing the sliding speed or increment in the sliding distance. Al 2 O 3 , B 4 C, and SiC reinforced aluminium matrix composites were fabricated through stir casting and characterized for microstructure and interfacial reaction [10]. e investigators reported that the cast composites were subjected to hot extraction at 420°C with an extrusion ratio of 27 at a speed of 1 m/min to reduce the porosity and enhance the particle distribution in the aluminium matrix. ey reported that due to the addition of SiC particles, the grain became finer as seen in the microstructure. ey observed macropores trapped in the center of the cluster of particles and micropores in the aluminium matrix. ey further reported that the wettability of B 4 C was increasing in the air due to the formation of a layer of B 2 O 3 on the B 4 C particles. erefore, the distribution of B 4 C particles was better than that of SiC and Al 2 O 3 in the composites processed in air. e EDS spectrum shows the presence of O, C, Si, and Al in the interface reaction layer.
Leyland and Matthews [11] investigated the significance of hardness (H) and elastic modulus (E) in controlling the wear. ey proposed that there are evidences, which suggest that elastic modulus has an important effect on wear such as hardness. e investigators have suggested the concept of nanocomposite coatings having high H and low E for better toughness. So, the nanocomposite is considered better for optimizing the resistance against wear in industrial materials. ey also discussed the importance of elastic strain and fracture toughness to find the wear behaviour. In an investigation, Sharma et al. [12] examined the wear behaviour of hybrid aluminium alloy composites reinforced with SiC and RE (Rare Earth) mixture CeO 2 and La 2 O 3 through stir casting. ey reported that, about 2% of rare Earth content can enhance the ultimate tensile strength and microhardness of percentage elongation of Al6063. ey observed an improvement of about 42% in wear rate composites as compared to base alloys. e volume fraction or weight fraction of the reinforcement particles are also affecting the microstructure, mechanical properties, and wear resistance of the composites. Different investigators have taken different weight fractions of the reinforcement. Rajesh et al. [9] have taken 5%, 10%, and 15% of the reinforcement. Fenghong et al. [5] considered wt. fractions of the reinforcement as 10%, 15%, and 20%. In another investigation, 2%, 4%, 6%, and 8% wt. of reinforcement were taken for the fabrication of the Al6061 alloy composites [13]. e aim of this investigation is to synthesize and characterize the Al7075-B 4 C composites followed by a sliding wear test.
is investigation aims to synthesize MMCs with Al-7075 as matrix and boron carbide (B 4 C) as reinforcement with varying sizes through stir casting. e results were interpreted on the basis of optical microstructure, mechanical properties, and surface morphologies.

Materials.
In the present investigation, Al7075 has been selected as a matrix and B 4 C of average size 50 μm with 99.9% purity has been selected as reinforcement. e major constituents of Al7075 in wt.% are Zn 5.8%, Mg 2.4%, Cu 1.5%, Fe 0.2%, Cr 0.2%, and balance Al. e chemical analysis of the reinforcement is given in Table 1. 2 Advances in Materials Science and Engineering     [5,8,13]. Liquid aluminium alloy was superheated to a temperature of 750°C during the liquefying process. B 4 C was added to the required measurements of the molten metal and mixed with a stirrer at speed of 600 rpm as per the norms followed by Rajesh et al. [9]. e liquid Al7075-B 4 C was poured into a die and allowed to cool. e composites were then withdrawn from the die and the composites are shown in Figure 1.

Heat Treatment.
In the muffle furnace (Figure 2), the ascast samples were heat-treated up to 465°C for two hours. After 2 hrs of the solution treatment, the specimens were quenched in the water. ese were subject to age hardening at 120°C for five hours followed by air cooling.

Hardness Test.
e hardness of the composites was determined by using the Brinell hardness tester. e indenter used was of 2.5 mm diameter, and the major load was 187.5 kgf.

Wear Test.
A sliding wear test was performed on the advanced rotary tribometer manufactured by Ducom, Bangalore, to assess the wear behaviour of the composites, as shown in Figure 3(a). A circular disc made of austenitic stainless steel (SS-304) was the wear disc used in the tribometer. e disc thickness and diameter were 60 mm and 10 mm, respectively. e wear diameter has been fixed at 40 mm. e hardness of the disc was 65 HRC. e specimens for the wear test were made (Figure 3(b)). e wear tests were conducted as per the standard of ASTM G99-05.

Microstructural and EDS Analysis.
e microstructure of the fabricated composites in as-cast and age-hardened conditions is shown in Figure 4. From the microstructure of the ascast composites, the same micropores are seen in Figures 4(b)-4(e) as compared to pure aluminium alloy (Figure 4(a)),   Al7075-10% B 4 C composite, and all age-hardened composites. is observation is in agreement with those reported by Rajesh et al. [9]. It is also seen that Al7075-10% B 4 C composite shows uniform distribution of the B 4 C particles as compared to others in which clusters of particles are seen. Due to age hardening, there is a refining of the grains as well as reduction of pores.
To identify the elemental composition of the compounds of the composites, EDS of the composites in cast condition was performed ( Figure 5). e EDS analysis indicates the composition of mainly Al7075 alloy along with some boron carbides. is observation is similar to those reported by Rajesh et al. [9] (Figure 4).

3.2.
Hardness. Ten positions were used for each component on the as-cast and age-hardened specimens. e average of all the results was considered and shown in Figure 6. In Figure 6, it can be observed that due to the addition of B 4 C particles to the Al7075, there is an increment of hardness. However, further increment in hardness is very less with increasing the wt.% of the reinforcement. ese results are in agreement with those reported by Rajesh et al. [9] in which hardness was increasing with 10% reinforcement and then decreasing. From Figure 6, it is observed that there is an increase in hardness due to age hardening in the composites. ese results are similar to those reported by Rajesh et al. [9].

Effect of Age Hardening and As-Cast Conditions on the Wear
Rate. e wear tests of the composites both as-cast and age-hardened were performed for a sliding speed of 1.5 m/s, 2.5 m/s, and 3.5 m/s and with varying load. e results are shown in Figures 7-9. From the results, it is observed that the wear resistance of the composites is    Advances in Materials Science and Engineering increasing with an increase in the volume fraction of the reinforcements. e wear resistance further increases due to age hardening. ese results are in agreement with those investigated by Rajesh et al. [9]. e increase in wear resistance in age-hardened specimens is may be due to the elimination of voids or porosity. From Figures 6-9, it can be observed that the wear rate is decreasing with an increase in hardness, and it is in agreement with findings from Rajesh et al. [9] in which they proposed that hard reinforcement particulate is restricting the composites from getting soft and resulting in reduced wear rate. e lower wear rate of the composites is also because of fine grains and almost uniform distribution of the reinforcement, as shown in Figure 4.

Worn Surface.
e surface morphologies of the as-cast and age-hardened Al7075/B 4 C AMMCs, taken with field emission scanning electron microscopy (FESEM), are shown in Figures 10(a)-10  micrographs, it is observed that as-cast AMMCs are having more craters as compared to age-hardened AMMCs. Larger grooves are seen in the as-cast AMMCs which indicate that there is more wear rate in as-cast AMMCs. From the FESEMs of as-cast wear surfaces, it is seen that the grooves are becoming smaller and smaller with the increase in the reinforcement. e surface morphologies of age-hardened samples show that there is no significant difference with an increase in reinforcement.
erefore, it can be concluded that the wear resistance can be improved by age hardening of the prepared composites.

Conclusions
e Al7075/B 4 C (50 μm) composites were fabricated by stir casting using a vacuum furnace. e characterization of composites with different weight fractions of reinforcement materials (6,8,10, and 12 wt.% of reinforcements) is carried out. e following findings are observed: (i) e microstructural study shows the homogeneous distribution of the reinforcement particles in the Al7075/B 4 C composites and reduction in the porosity in the age-hardened Al7075/B 4 C composites as compared to as-cast Al7075/B 4 C composites (ii) e age-hardened Al7075/B 4 C composites show higher hardness and wear resistance as compared to as-cast Al7075/B 4 C composites (iii) e wear resistance of the composite is dependent on the sliding speed, applied load, microstructure, weight percentage of the reinforcement, and age hardening (iv) e surface morphologies of the wear surfaces indicate that the presence of larger grooves means lower wear resistance of the composites erefore, the age hardening of the composites is recommended to further enhance the wear resistance.

Data Availability
e data used to support the findings of this study are available from the corresponding author upon request.

Conflicts of Interest
e authors declare that they have no known conflicts of interest or personal relationships that could have appeared to influence the work reported in this paper.